#------------------------------------------------------------------------------
#$Date: 2021-05-04 03:49:28 +0300 (Tue, 04 May 2021) $
#$Revision: 264820 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/38/4003899.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003899
loop_
_publ_author_name
'Smart, Megan M.'
'Smith Pellizzeri, Tiffany M.'
'Morrison, Gregory'
'McMillen, Colin D.'
'zur Loye, Hans-Conrad'
'Kolis, Joseph W.'
_publ_section_title
;
 Ferrite Materials Containing Kagomé Layers: Chemistry of Ba2Fe11Ge2O22
 and K2Co4V9O22 Hexaferrites
;
_journal_issue                   7
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2258
_journal_page_last               2266
_journal_paper_doi               10.1021/acs.chemmater.0c03852
_journal_volume                  33
_journal_year                    2021
_chemical_formula_sum            'Co4 K2 O22 V9'
_chemical_formula_weight         1124.38
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.8392(3)
_cell_length_b                   5.8392(3)
_cell_length_c                   14.5176(8)
_cell_measurement_reflns_used    6664
_cell_measurement_temperature    299(2)
_cell_measurement_theta_max      30.49
_cell_measurement_theta_min      2.81
_cell_volume                     428.68(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX3'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick 2014)'
_computing_structure_solution    'SHELXT-2014 (Sheldrick 2014)'
_diffrn_ambient_temperature      299(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Bruker D8 Venture Photon 100'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0285
_diffrn_reflns_av_unetI/netI     0.0120
_diffrn_reflns_Laue_measured_fraction_full 0.986
_diffrn_reflns_Laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            6107
_diffrn_reflns_point_group_measured_fraction_full 0.986
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.499
_diffrn_reflns_theta_min         2.806
_diffrn_source                   'Incoatec I\mS'
_exptl_absorpt_coefficient_mu    9.017
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.816
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS, Bruker'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.355
_exptl_crystal_description       plate
_exptl_crystal_F_000             529
_exptl_crystal_size_max          0.160
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.120
_refine_diff_density_max         0.842
_refine_diff_density_min         -0.699
_refine_diff_density_rms         0.139
_refine_ls_extinction_coef       0.053(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.215
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     46
_refine_ls_number_reflns         398
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.215
_refine_ls_R_factor_all          0.0215
_refine_ls_R_factor_gt           0.0213
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0234P)²+2.1368P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0601
_refine_ls_wR_factor_ref         0.0602
_reflns_Friedel_coverage         0.000
_reflns_number_gt                392
_reflns_number_total             398
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cm0c03852_si_002.cif
_cod_data_source_block           KCoV
_cod_depositor_comments
'Adding full bibliography for 4003899--4003900.cif.'
_cod_original_cell_volume        428.68(5)
_cod_database_code               4003899
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.326
_shelx_estimated_absorpt_t_max   0.411
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K 1.3333 1.6667 1.06299(13) 0.0186(4) Uani 1 6 d S T P . .
Co1 Co 0.3333 0.6667 0.81882(7) 0.0076(3) Uani 1 6 d S T P . .
V2 V 0.82238(7) 0.64476(14) 0.67032(4) 0.0052(3) Uani 1 2 d S T P . .
V3 V 0.0000 0.0000 0.5000 0.0055(4) Uani 1 12 d S T P . .
Co4 Co 0.6667 0.3333 0.45116(7) 0.0071(3) Uani 1 6 d S T P . .
V5 V 1.0000 1.0000 0.86668(8) 0.0065(3) Uani 1 6 d S T P . .
O1 O 0.6667 0.3333 0.5870(4) 0.0114(11) Uani 1 6 d S T P . .
O2 O 1.0000 1.0000 0.7405(3) 0.0087(11) Uani 1 6 d S T P . .
O3 O 0.2963(6) 0.1482(3) 0.41499(19) 0.0095(6) Uani 1 2 d S T P . .
O4 O 0.5022(3) 0.4978(3) 0.7367(2) 0.0160(7) Uani 1 2 d S T P . .
O5 O 1.1604(3) 1.3208(6) 0.9004(2) 0.0126(7) Uani 1 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 K1 O5 62.08(11) . 3_685 ?
O5 K1 O5 62.08(11) . 2_875 ?
O5 K1 O5 62.08(11) 3_685 2_875 ?
O5 K1 O5 99.00(6) . 7_887 ?
O5 K1 O5 130.13(6) 3_685 7_887 ?
O5 K1 O5 68.29(10) 2_875 7_887 ?
O5 K1 O5 68.29(10) . 8_567 ?
O5 K1 O5 130.13(6) 3_685 8_567 ?
O5 K1 O5 99.00(6) 2_875 8_567 ?
O5 K1 O5 61.37(13) 7_887 8_567 ?
O5 K1 O5 130.13(6) . 9_767 ?
O5 K1 O5 99.00(6) 3_685 9_767 ?
O5 K1 O5 68.30(11) 2_875 9_767 ?
O5 K1 O5 56.50(13) 7_887 9_767 ?
O5 K1 O5 116.87(4) 8_567 9_767 ?
O5 K1 O5 68.29(11) . 9_657 ?
O5 K1 O5 99.00(6) 3_685 9_657 ?
O5 K1 O5 130.13(6) 2_875 9_657 ?
O5 K1 O5 116.87(4) 7_887 9_657 ?
O5 K1 O5 56.50(13) 8_567 9_657 ?
O5 K1 O5 159.24(13) 9_767 9_657 ?
O5 K1 O5 130.13(6) . 8_577 ?
O5 K1 O5 68.30(10) 3_685 8_577 ?
O5 K1 O5 99.00(6) 2_875 8_577 ?
O5 K1 O5 116.87(4) 7_887 8_577 ?
O5 K1 O5 159.24(13) 8_567 8_577 ?
O5 K1 O5 61.37(13) 9_767 8_577 ?
O5 K1 O5 116.87(4) 9_657 8_577 ?
O5 K1 O5 99.00(6) . 7_787 ?
O5 K1 O5 68.30(10) 3_685 7_787 ?
O5 K1 O5 130.13(6) 2_875 7_787 ?
O5 K1 O5 159.24(13) 7_887 7_787 ?
O5 K1 O5 116.87(4) 8_567 7_787 ?
O5 K1 O5 116.87(4) 9_767 7_787 ?
O5 K1 O5 61.37(13) 9_657 7_787 ?
O5 K1 O5 56.50(13) 8_577 7_787 ?
O5 K1 O4 123.34(7) . 7_777 ?
O5 K1 O4 173.23(9) 3_685 7_777 ?
O5 K1 O4 123.34(7) 2_875 7_777 ?
O5 K1 O4 55.04(7) 7_887 7_777 ?
O5 K1 O4 55.04(7) 8_567 7_777 ?
O5 K1 O4 80.45(6) 9_767 7_777 ?
O5 K1 O4 80.45(6) 9_657 7_777 ?
O5 K1 O4 105.84(8) 8_577 7_777 ?
O5 K1 O4 105.84(8) 7_787 7_777 ?
O5 K1 O4 173.23(10) . 8_677 ?
O5 K1 O4 123.34(7) 3_685 8_677 ?
O5 K1 O4 123.34(7) 2_875 8_677 ?
O5 K1 O4 80.45(6) 7_887 8_677 ?
O5 K1 O4 105.84(8) 8_567 8_677 ?
O5 K1 O4 55.04(7) 9_767 8_677 ?
O5 K1 O4 105.84(8) 9_657 8_677 ?
O5 K1 O4 55.04(7) 8_577 8_677 ?
O5 K1 O4 80.45(6) 7_787 8_677 ?
O4 K1 O4 50.93(9) 7_777 8_677 ?
O5 K1 O4 123.34(7) . 9_667 ?
O5 K1 O4 123.34(7) 3_685 9_667 ?
O5 K1 O4 173.23(10) 2_875 9_667 ?
O5 K1 O4 105.84(8) 7_887 9_667 ?
O5 K1 O4 80.45(6) 8_567 9_667 ?
O5 K1 O4 105.84(8) 9_767 9_667 ?
O5 K1 O4 55.04(7) 9_657 9_667 ?
O5 K1 O4 80.45(6) 8_577 9_667 ?
O5 K1 O4 55.04(7) 7_787 9_667 ?
O4 K1 O4 50.93(9) 7_777 9_667 ?
O4 K1 O4 50.93(10) 8_677 9_667 ?
O4 Co1 O4 90.46(13) . 3_565 ?
O4 Co1 O4 90.46(13) . 2_665 ?
O4 Co1 O4 90.46(12) 3_565 2_665 ?
O4 Co1 O5 179.17(12) . 3_575 ?
O4 Co1 O5 88.96(9) 3_565 3_575 ?
O4 Co1 O5 88.96(9) 2_665 3_575 ?
O4 Co1 O5 88.96(9) . 2_765 ?
O4 Co1 O5 179.17(12) 3_565 2_765 ?
O4 Co1 O5 88.96(9) 2_665 2_765 ?
O5 Co1 O5 91.62(12) 3_575 2_765 ?
O4 Co1 O5 88.96(9) . 1_445 ?
O4 Co1 O5 88.96(9) 3_565 1_445 ?
O4 Co1 O5 179.17(12) 2_665 1_445 ?
O5 Co1 O5 91.62(12) 3_575 1_445 ?
O5 Co1 O5 91.62(12) 2_765 1_445 ?
O4 Co1 K1 124.94(9) . 1_445 ?
O4 Co1 K1 124.94(9) 3_565 1_445 ?
O4 Co1 K1 124.94(9) 2_665 1_445 ?
O5 Co1 K1 55.89(8) 3_575 1_445 ?
O5 Co1 K1 55.89(9) 2_765 1_445 ?
O5 Co1 K1 55.89(9) 1_445 1_445 ?
O4 Co1 K1 61.91(9) . 7_777 ?
O4 Co1 K1 128.686(17) 3_565 7_777 ?
O4 Co1 K1 128.686(17) 2_665 7_777 ?
O5 Co1 K1 118.91(10) 3_575 7_777 ?
O5 Co1 K1 51.44(2) 2_765 7_777 ?
O5 Co1 K1 51.44(2) 1_445 7_777 ?
K1 Co1 K1 63.03(3) 1_445 7_777 ?
O4 Co1 K1 128.687(17) . 7_787 ?
O4 Co1 K1 128.687(17) 3_565 7_787 ?
O4 Co1 K1 61.91(9) 2_665 7_787 ?
O5 Co1 K1 51.44(2) 3_575 7_787 ?
O5 Co1 K1 51.44(2) 2_765 7_787 ?
O5 Co1 K1 118.91(10) 1_445 7_787 ?
K1 Co1 K1 63.03(3) 1_445 7_787 ?
K1 Co1 K1 101.04(4) 7_777 7_787 ?
O4 Co1 K1 128.687(17) . 7_677 ?
O4 Co1 K1 61.91(9) 3_565 7_677 ?
O4 Co1 K1 128.687(17) 2_665 7_677 ?
O5 Co1 K1 51.44(2) 3_575 7_677 ?
O5 Co1 K1 118.91(10) 2_765 7_677 ?
O5 Co1 K1 51.44(2) 1_445 7_677 ?
K1 Co1 K1 63.03(3) 1_445 7_677 ?
K1 Co1 K1 101.04(4) 7_777 7_677 ?
K1 Co1 K1 101.03(4) 7_787 7_677 ?
O4 V2 O4 99.7(2) 3_665 . ?
O4 V2 O1 89.92(10) 3_665 . ?
O4 V2 O1 89.92(10) . . ?
O4 V2 O2 95.20(10) 3_665 . ?
O4 V2 O2 95.20(10) . . ?
O1 V2 O2 172.05(17) . . ?
O4 V2 O3 91.47(14) 3_665 8_666 ?
O4 V2 O3 168.69(13) . 8_666 ?
O1 V2 O3 92.10(11) . 8_666 ?
O2 V2 O3 81.71(11) . 8_666 ?
O4 V2 O3 168.69(13) 3_665 7_666 ?
O4 V2 O3 91.47(13) . 7_666 ?
O1 V2 O3 92.10(11) . 7_666 ?
O2 V2 O3 81.71(11) . 7_666 ?
O3 V2 O3 77.33(17) 8_666 7_666 ?
O4 V2 V2 92.34(9) 3_665 2_655 ?
O4 V2 V2 43.67(7) . 2_655 ?
O1 V2 V2 46.63(9) . 2_655 ?
O2 V2 V2 138.87(8) . 2_655 ?
O3 V2 V2 138.51(6) 8_666 2_655 ?
O3 V2 V2 97.14(8) 7_666 2_655 ?
O4 V2 V2 43.67(7) 3_665 3_665 ?
O4 V2 V2 92.34(9) . 3_665 ?
O1 V2 V2 46.63(9) . 3_665 ?
O2 V2 V2 138.86(8) . 3_665 ?
O3 V2 V2 97.14(8) 8_666 3_665 ?
O3 V2 V2 138.51(6) 7_666 3_665 ?
V2 V2 V2 60.0 2_655 3_665 ?
O4 V2 V3 130.15(10) 3_665 1_665 ?
O4 V2 V3 130.15(10) . 1_665 ?
O1 V2 V3 88.47(12) . 1_665 ?
O2 V2 V3 83.58(12) . 1_665 ?
O3 V2 V3 38.86(8) 8_666 1_665 ?
O3 V2 V3 38.86(8) 7_666 1_665 ?
V2 V2 V3 120.601(10) 2_655 1_665 ?
V2 V2 V3 120.601(10) 3_665 1_665 ?
O4 V2 V2 136.33(7) 3_665 3_675 ?
O4 V2 V2 87.66(9) . 3_675 ?
O1 V2 V2 133.38(9) . 3_675 ?
O2 V2 V2 41.13(8) . 3_675 ?
O3 V2 V2 82.86(8) 8_666 3_675 ?
O3 V2 V2 41.50(6) 7_666 3_675 ?
V2 V2 V2 120.0 2_655 3_675 ?
V2 V2 V2 180.0 3_665 3_675 ?
V3 V2 V2 59.401(10) 1_665 3_675 ?
O4 V2 V2 87.66(9) 3_665 2_765 ?
O4 V2 V2 136.33(7) . 2_765 ?
O1 V2 V2 133.38(9) . 2_765 ?
O2 V2 V2 41.13(8) . 2_765 ?
O3 V2 V2 41.50(6) 8_666 2_765 ?
O3 V2 V2 82.87(8) 7_666 2_765 ?
V2 V2 V2 180.0 2_655 2_765 ?
V2 V2 V2 120.0 3_665 2_765 ?
V3 V2 V2 59.401(10) 1_665 2_765 ?
V2 V2 V2 60.0 3_675 2_765 ?
O3 V3 O3 180.00(13) 8_556 2 ?
O3 V3 O3 96.10(13) 8_556 . ?
O3 V3 O3 83.90(13) 2 . ?
O3 V3 O3 83.90(13) 8_556 9_556 ?
O3 V3 O3 96.10(13) 2 9_556 ?
O3 V3 O3 96.10(13) . 9_556 ?
O3 V3 O3 96.10(13) 8_556 3 ?
O3 V3 O3 83.90(13) 2 3 ?
O3 V3 O3 83.90(13) . 3 ?
O3 V3 O3 180.0 9_556 3 ?
O3 V3 O3 83.90(13) 8_556 7_556 ?
O3 V3 O3 96.10(13) 2 7_556 ?
O3 V3 O3 180.0 . 7_556 ?
O3 V3 O3 83.90(13) 9_556 7_556 ?
O3 V3 O3 96.10(13) 3 7_556 ?
O3 V3 V2 86.52(9) 8_556 3_565 ?
O3 V3 V2 93.48(9) 2 3_565 ?
O3 V3 V2 137.83(6) . 3_565 ?
O3 V3 V2 42.17(6) 9_556 3_565 ?
O3 V3 V2 137.83(6) 3 3_565 ?
O3 V3 V2 42.17(6) 7_556 3_565 ?
O3 V3 V2 93.48(9) 8_556 9_546 ?
O3 V3 V2 86.52(9) 2 9_546 ?
O3 V3 V2 42.17(6) . 9_546 ?
O3 V3 V2 137.83(6) 9_556 9_546 ?
O3 V3 V2 42.17(6) 3 9_546 ?
O3 V3 V2 137.83(6) 7_556 9_546 ?
V2 V3 V2 180.000(14) 3_565 9_546 ?
O3 V3 V2 42.17(6) 8_556 2_655 ?
O3 V3 V2 137.83(6) 2 2_655 ?
O3 V3 V2 93.48(9) . 2_655 ?
O3 V3 V2 42.17(6) 9_556 2_655 ?
O3 V3 V2 137.83(6) 3 2_655 ?
O3 V3 V2 86.52(9) 7_556 2_655 ?
V2 V3 V2 61.20(2) 3_565 2_655 ?
V2 V3 V2 118.80(2) 9_546 2_655 ?
O3 V3 V2 137.83(6) 8_556 8_456 ?
O3 V3 V2 42.17(6) 2 8_456 ?
O3 V3 V2 86.52(9) . 8_456 ?
O3 V3 V2 137.83(6) 9_556 8_456 ?
O3 V3 V2 42.17(6) 3 8_456 ?
O3 V3 V2 93.48(9) 7_556 8_456 ?
V2 V3 V2 118.80(2) 3_565 8_456 ?
V2 V3 V2 61.20(2) 9_546 8_456 ?
V2 V3 V2 180.0 2_655 8_456 ?
O3 V3 V2 42.17(6) 8_556 1_445 ?
O3 V3 V2 137.83(6) 2 1_445 ?
O3 V3 V2 137.83(6) . 1_445 ?
O3 V3 V2 86.52(9) 9_556 1_445 ?
O3 V3 V2 93.48(9) 3 1_445 ?
O3 V3 V2 42.17(6) 7_556 1_445 ?
V2 V3 V2 61.20(2) 3_565 1_445 ?
V2 V3 V2 118.80(2) 9_546 1_445 ?
V2 V3 V2 61.20(2) 2_655 1_445 ?
V2 V3 V2 118.80(2) 8_456 1_445 ?
O3 V3 V2 137.83(6) 8_556 7_666 ?
O3 V3 V2 42.17(6) 2 7_666 ?
O3 V3 V2 42.17(6) . 7_666 ?
O3 V3 V2 93.48(9) 9_556 7_666 ?
O3 V3 V2 86.52(9) 3 7_666 ?
O3 V3 V2 137.83(6) 7_556 7_666 ?
V2 V3 V2 118.80(2) 3_565 7_666 ?
V2 V3 V2 61.20(2) 9_546 7_666 ?
V2 V3 V2 118.80(2) 2_655 7_666 ?
V2 V3 V2 61.20(2) 8_456 7_666 ?
V2 V3 V2 180.0 1_445 7_666 ?
O3 Co4 O3 113.00(8) . 3_665 ?
O3 Co4 O3 113.00(8) . 2_655 ?
O3 Co4 O3 112.99(8) 3_665 2_655 ?
O3 Co4 O1 105.66(9) . . ?
O3 Co4 O1 105.66(9) 3_665 . ?
O3 Co4 O1 105.66(9) 2_655 . ?
O5 V5 O5 112.00(9) 2_765 . ?
O5 V5 O5 112.00(10) 2_765 3_675 ?
O5 V5 O5 112.00(10) . 3_675 ?
O5 V5 O2 106.80(11) 2_765 . ?
O5 V5 O2 106.80(11) . . ?
O5 V5 O2 106.80(11) 3_675 . ?
O5 V5 K1 146.35(12) 2_765 7_887 ?
O5 V5 K1 57.19(2) . 7_887 ?
O5 V5 K1 57.19(2) 3_675 7_887 ?
O2 V5 K1 106.85(4) . 7_887 ?
O5 V5 K1 57.19(2) 2_765 7_777 ?
O5 V5 K1 146.35(12) . 7_777 ?
O5 V5 K1 57.19(2) 3_675 7_777 ?
O2 V5 K1 106.85(3) . 7_777 ?
K1 V5 K1 111.96(3) 7_887 7_777 ?
O5 V5 K1 57.19(2) 2_765 7_787 ?
O5 V5 K1 57.19(2) . 7_787 ?
O5 V5 K1 146.35(12) 3_675 7_787 ?
O2 V5 K1 106.85(3) . 7_787 ?
K1 V5 K1 111.96(3) 7_887 7_787 ?
K1 V5 K1 111.96(3) 7_777 7_787 ?
Co4 O1 V2 127.53(12) . . ?
Co4 O1 V2 127.53(12) . 2_655 ?
V2 O1 V2 86.75(17) . 2_655 ?
Co4 O1 V2 127.53(12) . 3_665 ?
V2 O1 V2 86.75(17) . 3_665 ?
V2 O1 V2 86.75(17) 2_655 3_665 ?
V5 O2 V2 119.58(12) . 3_675 ?
V5 O2 V2 119.58(12) . 2_765 ?
V2 O2 V2 97.73(16) 3_675 2_765 ?
V5 O2 V2 119.58(12) . . ?
V2 O2 V2 97.73(16) 3_675 . ?
V2 O2 V2 97.73(16) 2_765 . ?
V3 O3 Co4 124.86(15) . . ?
V3 O3 V2 98.97(11) . 9_546 ?
Co4 O3 V2 116.06(11) . 9_546 ?
V3 O3 V2 98.97(11) . 7_666 ?
Co4 O3 V2 116.06(11) . 7_666 ?
V2 O3 V2 97.01(12) 9_546 7_666 ?
V2 O4 V2 92.65(14) 2_655 . ?
V2 O4 Co1 132.34(8) 2_655 . ?
V2 O4 Co1 132.34(8) . . ?
V2 O4 K1 102.27(11) 2_655 7_777 ?
V2 O4 K1 102.27(11) . 7_777 ?
Co1 O4 K1 84.83(10) . 7_777 ?
V5 O5 Co1 129.08(17) . 1_665 ?
V5 O5 K1 143.35(16) . . ?
Co1 O5 K1 87.57(11) 1_665 . ?
V5 O5 K1 94.14(7) . 7_887 ?
Co1 O5 K1 94.74(7) 1_665 7_887 ?
K1 O5 K1 81.00(6) . 7_887 ?
V5 O5 K1 94.14(7) . 7_787 ?
Co1 O5 K1 94.74(7) 1_665 7_787 ?
K1 O5 K1 81.00(6) . 7_787 ?
K1 O5 K1 159.24(13) 7_887 7_787 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K1 O5 2.937(4) . ?
K1 O5 2.938(4) 3_685 ?
K1 O5 2.938(4) 2_875 ?
K1 O5 2.9682(6) 7_887 ?
K1 O5 2.9682(6) 8_567 ?
K1 O5 2.9682(6) 9_767 ?
K1 O5 2.9682(6) 9_657 ?
K1 O5 2.9682(6) 8_577 ?
K1 O5 2.9682(6) 7_787 ?
K1 O4 3.351(3) 7_777 ?
K1 O4 3.351(3) 8_677 ?
K1 O4 3.351(4) 9_667 ?
Co1 O4 2.083(3) . ?
Co1 O4 2.083(3) 3_565 ?
Co1 O4 2.083(3) 2_665 ?
Co1 O5 2.112(3) 3_575 ?
Co1 O5 2.113(3) 2_765 ?
Co1 O5 2.113(3) 1_445 ?
Co1 K1 3.545(2) 1_445 ?
Co1 K1 3.7827(10) 7_777 ?
Co1 K1 3.7828(10) 7_787 ?
Co1 K1 3.7828(10) 7_677 ?
V2 O4 1.886(2) 3_665 ?
V2 O4 1.886(2) . ?
V2 O1 1.986(3) . ?
V2 O2 2.066(3) . ?
V2 O3 2.077(2) 8_666 ?
V2 O3 2.077(2) 7_666 ?
V2 V2 2.7277(12) 2_655 ?
V2 V2 2.7277(12) 3_665 ?
V2 V3 3.0563(7) 1_665 ?
V2 V2 3.1115(12) 3_675 ?
V2 V2 3.1115(12) 2_765 ?
V3 O3 1.941(3) 8_556 ?
V3 O3 1.941(3) 2 ?
V3 O3 1.941(3) . ?
V3 O3 1.941(3) 9_556 ?
V3 O3 1.941(3) 3 ?
V3 O3 1.941(3) 7_556 ?
V3 V2 3.0563(7) 3_565 ?
V3 V2 3.0563(7) 9_546 ?
V3 V2 3.0563(7) 2_655 ?
V3 V2 3.0563(7) 8_456 ?
V3 V2 3.0563(7) 1_445 ?
V3 V2 3.0563(7) 7_666 ?
Co4 O3 1.945(3) . ?
Co4 O3 1.945(3) 3_665 ?
Co4 O3 1.945(3) 2_655 ?
Co4 O1 1.972(5) . ?
V5 O5 1.695(3) 2_765 ?
V5 O5 1.695(3) . ?
V5 O5 1.695(3) 3_675 ?
V5 O2 1.831(5) . ?
V5 K1 3.5224(7) 7_887 ?
V5 K1 3.5224(7) 7_777 ?
V5 K1 3.5225(7) 7_787 ?
O1 V2 1.986(3) 2_655 ?
O1 V2 1.986(3) 3_665 ?
O2 V2 2.066(3) 3_675 ?
O2 V2 2.066(3) 2_765 ?
O3 V2 2.077(2) 9_546 ?
O3 V2 2.077(2) 7_666 ?
O4 V2 1.886(2) 2_655 ?
O4 K1 3.351(3) 7_777 ?
O5 Co1 2.113(3) 1_665 ?
O5 K1 2.9681(6) 7_887 ?
O5 K1 2.9682(6) 7_787 ?
